|Year : 2018 | Volume
| Issue : 3 | Page : 166-172
Microhardness of different esthetic restorative materials: Evaluation and comparison after exposure to acidic drink
Claudio Poggio, Matteo Viola, Maria Mirando, Marco Chiesa, Riccardo Beltrami, Marco Colombo
Department of Clinical, Surgical, Diagnostic and Pediatric Sciences, Section of Dentistry, University of Pavia, Pavia, Italy
|Date of Web Publication||4-May-2018|
Prof. Claudio Poggio
Department of Clinical, Surgical, Diagnostic and Pediatric Sciences, Section of Dentistry, Policlinico “San Matteo”, Piazzale Golgi 3, 27100 Pavia
Source of Support: None, Conflict of Interest: None
Background: Acidic beverages, such as soft drinks (orange juice and cola), can produce erosion of resin composites. The aim of this in vitro study was to evaluate the effect of immersion in acidic drink on the Vickers microhardness (VK) of different esthetic restorative materials (one nanohybrid Ormocer-based composite, one nanoceramic composite, one nanofilled composite, and one microfilled hybrid composite).
Materials and Methods: In this in vitro study, thirty specimens of each esthetic restorative material were divided into three subgroups (n = 10): specimens of group 1 were used as control, specimens of group 2 were immersed in 50 ml of acidic drink for 1 day, specimens of group 3 were immersed in 50 ml of acidic drink for 7 days. Data were analyzed by Shapiro–Wilk test to assess the normality of the distributions followed by nonparametric Kruskal–Wallis analysis of variance and Mann–Whitney U-test comparison test among groups. A significant level of α = 0.05 was set for comparison between the groups.
Results: Mann–Whitney U-test showed that each material showed lower microhardness values after immersion in acidic solution (P < 0.05). Paired t-test confirmed that microhardness for each composite did not change after immersion in distilled water (Control group) (P > 0.05). Significant changes were registered for all restorative materials after immersion in acidic solution for 1 day and 7 days (P < 0.05).
Conclusion: The Filtek Supreme XTE, a nanofilled composite, and Admira Fusion, a nanohybrid ormocer-based composite, showed the best behavior. The Ceram X Universal (nanoceramic composite) although reached lower hardness values than the previous materials, but resisted well to the 1 week immersion in soft-drink. Finally, the Gradia Direct achieved the most disappointing results: Low microhardness values are justified by the nature of its filling (microfilled hybrid composite).
Keywords: Acidic, drink, erosion, hardness, restorative materials
|How to cite this article:|
Poggio C, Viola M, Mirando M, Chiesa M, Beltrami R, Colombo M. Microhardness of different esthetic restorative materials: Evaluation and comparison after exposure to acidic drink. Dent Res J 2018;15:166-72
|How to cite this URL:|
Poggio C, Viola M, Mirando M, Chiesa M, Beltrami R, Colombo M. Microhardness of different esthetic restorative materials: Evaluation and comparison after exposure to acidic drink. Dent Res J [serial online] 2018 [cited 2018 May 27];15:166-72. Available from: http://www.drjjournal.net/text.asp?2018/15/3/166/231863
| Introduction|| |
Resin-based composites are used worldwide in dentistry, mainly because of their esthetic quality and good physical properties. Since resin composites were first developed, many efforts have been made to improve the clinical behavior of this restorative material.
Resin composites have been classified according to various characteristics, such as size, content, and filler type, and the physical and mechanical properties of the materials. Nanotechnology, known as molecular nanotechnology, is the production of functional materials and structures, at a range of 0.1–100 nm, by various physical and chemical methods. A nanohybrid is a hybrid resin composite with nanofiller in a prepolymerized filler form, whereas nanofill is a composite resin that is composed of both nanomers and nanoclusters. The term Ormocer is an abbreviation for Organically Modified Ceramics. Ormocers were initially used together with dimethacrylates, but a recent material formulated with a pure-Ormocer-based resin matrix has been developed. An Ormocer is a hybrid molecular structure. This combines organic and inorganic components at nanoscopic scale through the sol-gel method, and the main characteristic of this type of material is the incorporation of organic groups linked to the inorganic backbone. Ormocer materials contain inorganic-organic copolymers in addition to the inorganic silanated filler particles. Ormocers are described as three-dimensionally cross-linked copolymers. The Ormocer matrix is a polymer even before light curing. It consists of ceramic polysiloxane, which has low shrinkage as against the organic dimethacrylate monomer matrix seen in composites.
Acidic beverages, such as soft drinks (orange juice and cola), can produce erosion of resin composites., The surface degradation of resin materials is related to the content and distribution of the fillers, the composition of the matrix resin, and the effect of silane surface treatment on the fillers., Although the mechanical properties of these materials have been improved substantially, their antibacterial properties are still limited., The bacterial accumulation on the surfaces of restorative materials can provide the bacterial source leading to the development of secondary caries and periodontal diseases. Bacterial accumulation is highly dependent on the characteristics of the material surface, and the roughness of resin composites can influence the oral biofilm adherence. Biofilm formation is a stepwise process initiated by adhesion of planktonic bacteria onto the surface of a tooth or other structures in the oral cavity.
This process progresses from colonization and coadhesion, through growth and maturation, to detachment and spread of the microorganisms from the biofilm. The physical and chemical properties of the surface affect the feasibility of bacterial infection. Correlations between bacterial adhesion and various surface characteristics (chemical composition, surface energy, surface roughness, and presence of functional groups on the surface) have been intensively investigated in an attempt to reduce bacterial adhesion through surface modification.,
The aim of thisin vitro study was to evaluate the effect of immersion in acidic drink on the Vickers microhardness (VK) of different esthetic restorative materials (one nanohybrid Ormocer-based composite, one nanoceramic composite, one nanofilled composite, one microfilled hybrid composite).
| Materials and Methods|| |
In thisin vitro study, one nanohybrid Ormocer-based composite (Admira Fusion, Voco, Cuxhaven, Germany), one nanoceramic composite (Ceram X Universal, Dentsply De Trey, Konstanz, Germany), one nanofilled composite (Filtek Supreme XTE, 3M ESPE, St Paul, MN, USA), and one microfilled hybrid composite (Gradia Direct, GC Corporation, Tokyo, Japan); for each brand, the A3 Vita shade was selected [Table 1]. All materials were polymerized according to manufacturers' instructions into silicon rings (height 2 mm; internal diameter 6 mm; and external diameter 8 mm) to obtain specimens of identical size. Cavities of these rings were slightly overfilled with the material, covered with Mylar strip (Henry Schein, Melville, NY, USA), pressed between glass plates and polymerized for 40 s on each side using a curing unit (Celalux II, Voco, Cuxhaven, Germany). One light polymerization mode was used for each material standard: 1000 mW/cm2 for 40 s. The intensity of the light was verified with a radiometer (SDS Kerr, Orange, CA, USA). The light was placed perpendicular to the specimen surface, at distance of 1.5 mm. The upper surface of each specimen was then polished with fine and superfine polishing disks (Sof-Lex Pop On; 3M ESPE, St. Paul, MN, USA) to simulate clinical conditions.
Thirty cylindrical specimens of each material were prepared in this manner. After polymerization and during the experimentation, the specimens were stored in distilled water at 37°C and 100% humidity before performing the Vickers hardness test.
Immersion in acidic drink
Specimens of each esthetic restorative material were divided into three subgroups (n = 10): specimens of group 1 were used as control, specimens of group 2 were immersed in 50 ml of acidic drink (Coca-Cola/Coca-Cola Company, Milano, Italy) for 1 day, specimens of group 3 were immersed in 50 ml of acidic drink (Coca-Cola/Coca-Cola Company, Milano, Italy) for 7 days.
Surface microhardness measurements
The VK of the enamel surface was determined with a microhardness tester (Isoscan HV 1OD, LTF SpA, Antegnate, BG, Italy) using a Vickers diamond indenter and a 100 g load applied for 20 s and a 40x objective lens at the baseline time and after the experimental stage. Five VK readings were recorded for each sample surface. Five indentations equally placed over a circle and each no closer than 0.5 mm to the adjacent indentations were made on the surface of each specimen.
For a given specimen, the five hardness values for each surface were averaged and reported as a single value. The diagonals' length of the indentations was measured by a built-in scaled microscope, and a Vickers values were converted into microhardness values. Microhardness was obtained using the following equation: VK = 1.854 P/d2, where VK is Vickers microhardness in kgf/mm2, P is the load in kgf and d is the length of the diagonals in mm.
The data were analyzed using Stata 12 software (Stata, College Station, Texas, USA). Descriptive statistics including the mean, standard error of mean, and minimum and maximum values were calculated for all groups. Statistical analysis of the results of microhardness testing included Shapiro-Wilk test to assess the normality of the distributions followed by nonparametric Kruskal-Wallis analysis of variance (ANOVA) and Mann-Whitney U comparison test among groups. A significant level of α = 0.05 was set for comparison between the groups. For each specimen microhardness before immersion was compared with a paired t-test with microhardness after immersion to define the amount of erosion.
| Results|| |
Descriptive statistics of the microhardness values are reported in [Table 2] and displayed in [Figure 1]. Baseline values are significantly different for each composite (P< 0.05). Data are not normally distributed as confirmed by Shapiro–Wilk test (P< 0.05). Kruskal–Wallis ANOVA confirmed significant differences in microhardness Vickers values among the three experimental groups (P< 0.05). Mann–Whitney U test showed that, except for control group, each composite showed lower microhardness values after immersion in acidic solution (P< 0.05). The lowest values were registered after immersion in acidic solution for 1 week (P< 0.05). Paired t-test confirmed that microhardness for each composite did not change after immersion in distilled water (control group) (P > 0.05). Significant changes were registered for all restorative materials after immersion in acidic solution for 1 day and 7 days (P< 0.05). [Figure 2], [Figure 3], [Figure 4], [Figure 5] show the gradual surface changes and indentations of the different esthetic restorative materials tested.
|Table 2: Mean±standard deviation surface microhardness values of tested restorative materials before and after immersion in solutions|
Click here to view
|Figure 1: Box-plots for Vickers microhardness of material tested for each experimental group. Bold horizontal line represents median.|
Click here to view
|Figure 2: Photomicrographs of Admira Fusion before and after immersion in acidic drink for 1 and 7 days (×40). (a and b) Before immersion; (c and d) after immersion in acidic drink for 1 day, (e and f) after immersion in acidic drink for 7 days.|
Click here to view
|Figure 3: Photomicrographs of Ceram X Universal before and after immersion in acidic drink for 1 and 7 days (×40). (a and b) Before immersion; (c and d) after immersion in acidic drink for 1 day, (e and f) after immersion in acidic drink for 7 days.|
Click here to view
|Figure 4: Photomicrographs of Filtek Supreme XTE before and after immersion in acidic drink for 1 and 7 days (×40). (a and b) Before immersion; (c and d) after immersion in acidic drink for 1 day, (e and f) after immersion in acidic drink for 7 days.|
Click here to view
|Figure 5: Photomicrographs of Gradia Direct before and after immersion in acidic drink for 1 and 7 days (×40). (a and b) Before immersion; (c and d) after immersion in acidic drink for 1 day, (e and f) after immersion in acidic drink for 7 days.|
Click here to view
| Discussion|| |
The use of resin-based restorative materials in dentistry has substantially increased over the past few years because of their good esthetic appearance, improvements in formulations, ease of handling, and ability to establish a bond to dental hard tissues.,, To be clinically successful, restorative materials are required to have long-term continuousness, a quality which is strongly influenced not only by the intrinsic characteristics of the materials but also by the environment to which they are exposed to., However, the oral cavity is a complex, aqueous environment where the restorative material is in contact with saliva. In addition, other factors such as low pH due to acidic foods and drinks may influence the material's mechanical and physical characteristics.
The consumption of sports and energy drinks has gained high popularity among the young population in recent years, but they are being widely consumed by the general population. In addition to erosion of tooth hard tissues, the erosion of restorative materials has also received attention from researchers.,, It has been shown that erosion induced substance loss, surface degradation, and reduced abrasive-resistance of restorative materials. Although restorative materials are less susceptible to erosive attacks compared to enamel, the erosive attack can induce, at least to some extent, the degradation of the matrix and fillers of restorative materials.
Even though a great variety of substances may be present at the oral environment, water, saliva, acids, bases, salts, and alcohols have been related to the reduction of hardness, flexural strength, and flexural modulus properties., In addition, the biofilm accumulated over the restoration can produce acidic substances that may imply surface degradation, leading to the material's softening and surface roughening  with regard to these acidic substances, the lactic, propionic, and acetic acids are commonly found in the oral environment and they are used as storage solutions for screening accelerated hydrolysis phenomena of composite resins  and increase of hygroscopic expansion of Bis-GMA-based materials. Chemical substances may affect more actively the organic matrix of composites, but the type, size, and concentration of fillers may also influence the material's resistance to degradation.
Thisin vitro study focused on Vickers microhardness (VK) of different esthetic restorative materials after exposure to acidic drink.
The material's hardness is one of the most important properties and correlates well with compressive strength, resistance to intraoral softening, and degree of conversion., A low surface hardness value is largely related to inadequate wear resistance  and proclivity to scratching, which can compromise fatigue strength and lead to failure of the restoration.
In the current study, Filtek Supreme XTE registered the highest values of microhardness but respectively showed quite higher percentage loss of microhardness after 1 week immersion in soft-drink. Conversely Gradia Direct registered the lowest values and after a week immersion in the acidic drink lost about 20% of its initial hardness. The nanoceramic composite (Ceram X Universal) presented initial hardness values which amount to 57 HV (less than the initial values of Admira and Filtek Supreme) but resisted acid attack successfully. Finally, the nanohybrid Ormocer-based composite (Admira Fusion), offered good initial values of microhardness and did not show a significant loss of microhardness after 1 week immersion in soft drink.
In a clinical environment, a material's decrease of hardness may contribute to its deterioration. Underin vivo conditions, composite resin materials may be exposed either discontinuously or continually to chemical agents found in saliva, food, and beverages. Consequently, in the short-or long-term, these conditions may have a different deleterious effect on the polymeric network, modifying its structure physically and chemically.
| Conclusion|| |
Despite the limitations of thisin vitro study, the composite that showed the best behavior both initial and after the acid attack is the Filtek Supreme XTE (nanofilled composite), followed by Admira Fusion (nanohybrid Ormocer-based composite). The Ceram X Universal (nanoceramic composite) although reached lower hardness values than the previous materials, but resisted well to the 1 week immersion in soft-drink. Finally, the product that achieved the most disappointing results is the Gradia Direct: Low microhardness values are justified by the nature of its filling (microfilled hybrid composite). Further investigations may be required to evaluate the effect of acidic solutions on mechanical and surface properties of esthetic restorative materials containing different types, sizes, and content of fillers.
The authors are grateful to LTF SpA Antegnate, Bg, Italy for surface microhardness measurements.
Financial support and sponsorship
Conflicts of interest
The authors of this manuscript declare that they have no conflicts of interest, real or perceived, financial or nonfinancial in this article.
| References|| |
de Alencar E Silva Leite ML, da Cunha Medeiros E Silva FD, Meireles SS, Duarte RM, Andrade AK. The effect of drinks on color stability and surface roughness of nanocomposites. Eur J Dent 2014;8:330-6.
Mitra SB, Wu D, Holmes BN. An application of nanotechnology in advanced dental materials. J Am Dent Assoc 2003;134:1382-90.
Senawongse P, Pongprueksa P. Surface roughness of nanofill and nanohybrid resin composites after polishing and brushing. J Esthet Restor Dent 2007;19:265-73.
Cunha LG, Alonso RC, Santos PH, Sinhoreti MA. Comparative study of the surface roughness of ormocer-based and conventional composites. J Appl Oral Sci 2003;11:348-53.
Bacchi A, Feitosa VP, da Silva Fonseca AS, Cavalcante LM, Silikas N, Schneider LF, et al.
Shrinkage, stress, and modulus of dimethacrylate, ormocer, and silorane composites. J Conserv Dent 2015;18:384-8.
] [Full text]
Kalra S, Singh A, Gupta M, Chadha V. Ormocer: An aesthetic direct restorative material; anin vitro
study comparing the marginal sealing ability of organically modified ceramics and a hybrid composite using an ormocer-based bonding agent and a conventional fifth-generation bonding agent. Contemp Clin Dent 2012;3:48-53.
] [Full text]
Fatima N, Abidi SY, Qazi FU, Jat SA. Effect of different tetra pack juices on microhardness of direct tooth colored-restorative materials. Saudi Dent J 2013;25:29-32.
Asmussen E. Softening of BISGMA-based polymers by ethanol and by organic acids of plaque. Scand J Dent Res 1984;92:257-61.
Lee SY, Greener EH, Mueller HJ, Chiu CH. Effect of food and oral simulating fluids on dentine bond and composite strength. J Dent 1994;22:352-9.
Montanaro L, Campoccia D, Rizzi S, Donati ME, Breschi L, Prati C, et al.
Evaluation of bacterial adhesion of Streptococcus mutans
on dental restorative materials. Biomaterials 2004;25:4457-63.
Cruz AD, Cogo K, Bergamaschi Cde C, Bóscolo FN, Groppo FC, Almeida SM, et al.
Oral Streptococci growth on aging and non-aging esthetic restorations after radiotherapy. Braz Dent J 2010;21:346-50.
Gyo M, Nikaido T, Okada K, Yamauchi J, Tagami J, Matin K, et al.
Surface response of fluorine polymer-incorporated resin composites to cariogenic biofilm adherence. Appl Environ Microbiol 2008;74:1428-35.
Bashetty K, Joshi S. The effect of one-step and multi-step polishing systems on surface texture of two different resin composites. J Conserv Dent 2010;13:34-8.
] [Full text]
Badra VV, Faraoni JJ, Ramos RP, Palma-Dibb RG. Influence of different beverages on the microhardness and surface roughness of resin composites. Oper Dent 2005;30:213-9.
de Moraes RR, Marimon JL, Schneider LF, Sinhoreti MA, Correr-Sobrinho L, Bueno M, et al.
Effects of 6 months of aging in water on hardness and surface roughness of two microhybrid dental composites. J Prosthodont 2008;17:323-6.
Erdemir U, Yildiz E, Eren MM, Ozel S. Surface hardness evaluation of different composite resin materials: Influence of sports and energy drinks immersion after a short-term period. J Appl Oral Sci 2013;21:124-31.
Okada K, Tosaki S, Hirota K, Hume WR. Surface hardness change of restorative filling materials stored in saliva. Dent Mater 2001;17:34-9.
Yap AU, Tan SH, Wee SS, Lee CW, Lim EL, Zeng KY, et al.
Chemical degradation of composite restoratives. J Oral Rehabil 2001;28:1015-21.
Rios D, Honório HM, Francisconi LF, Magalhães AC, de Andrade Moreira Machado MA, Buzalaf MA, et al
. In situ
effect of an erosive challenge on different restorative materials and on enamel adjacent to these materials. J Dent 2008;36:152-7.
Yu H, Wegehaupt FJ, Wiegand A, Roos M, Attin T, Buchalla W, et al.
Erosion and abrasion of tooth-colored restorative materials and human enamel. J Dent 2009;37:913-22.
Yu H, Buchalla W, Cheng H, Wiegand A, Attin T. Topical fluoride application is able to reduce acid susceptibility of restorative materials. Dent Mater J 2012;31:433-42.
Aliping-McKenzie M, Linden RW, Nicholson JW. The effect of Coca-Cola and fruit juices on the surface hardness of glass-ionomers and 'compomers'. J Oral Rehabil 2004;31:1046-52.
Almeida GS, Poskus LT, Guimarães JG, da Silva EM. The effect of mouthrinses on salivary sorption, solubility and surface degradation of a nanofilled and a hybrid resin composite. Oper Dent 2010;35:105-11.
Münchow EA, Ferreira AC, Machado RM, Ramos TS, Rodrigues-Junior SA, Zanchi CH, et al.
Effect of acidic solutions on the surface degradation of a micro-hybrid composite resin. Braz Dent J 2014;25:321-6.
Lee SY, Huang HM, Lin CY, Shih YH. Leached components from dental composites in oral simulating fluids and the resultant composite strengths. J Oral Rehabil 1998;25:575-88.
Cilli R, Pereira JC, Prakki A. Properties of dental resins submitted to pH catalysed hydrolysis. J Dent 2012;40:1144-50.
Uhl A, Mills RW, Jandt KD. Photoinitiator dependent composite depth of cure and Knoop hardness with halogen and LED light curing units. Biomaterials 2003;24:1787-95.
Say EC, Civelek A, Nobecourt A, Ersoy M, Guleryuz C. Wear and microhardness of different resin composite materials. Oper Dent 2003;28:628-34.
Suese K, Kawazoe T. Wear resistance of hybrid composite resin for crown material by the two-body sliding test. Dent Mater J 2002;21:225-37.
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5]
[Table 1], [Table 2]